Ⅱ. Study on Organic Solar Cells for Improving Performances
2.3. A Selenophene Analogue of PCDTBT: Selective Fine-Tuning of LUMO to Lower of
2.3.3 Results and Discussion
As shown in Figure 2.3.1a, the UV−vis absorption spectra of PCDSeBT both in chloroform solution and solid state exhibit two distinct absorption bands, as typically observed for donor (D)-acceptor (A) low bandgap materials. The absorption maxima (λmax) of the film are located at 403 and 589 nm. The shorter absorption band is due to π−π* transitions of the polymer backbone,141 while the lower-energy peak is attributed to intramolecular charge transfer (ICT) in the electron-rich and electron-deficient units.142,143 It is worth noting that the maxima absorption values of PCDSeBT in the film are slightly broadened without any obvious red-shift when compared to the solution. This verifies that only a small reorganization via π−π stacking between the polymer chains is within view during the film formation because of the interchain aggregates in solution.144 This observation is in contrast to many conjugated polymers, in which there is a red-shift that occurs in going from the solution to the solid state due to the aggregation of the polymer chains in the solid state,145 even the PCDTBT film is red-shifted by 30 nm vs solution. Besides, the deep blue color of PCDSeBT solution is observed unlike the red color of PCDTBT in solution (see the digital photograph in Figure 2.3.1a).
Figure 2. 3. 1. UV–vis absorption spectra of PCDSeBT in chloroform and the thin film on the quartz (a). Inset: images of PCDSeBT and PCDTBT in chloroform solutions. Cyclic voltammogram of PCDSeBT thin film (b). Energy-level diagrams of PCDSeBT and PCDTBT (c). Graphical representation of a methyl-substituted CDSeBT dimer (d).
Notably, although the absorption profile of PCDSeBT is similar to that of the thiophene analogue, PCDTBT, the absorption onset of PCDSeBT is significantly red-shifted by ∼70 nm, corresponding to a lower optical bandgap (Eg opt = 1.70 eV) than PCDTBT (Eg opt = 1.85 eV). This apparently demonstrates that, in agreement with earlier studies and experimental studies,146,147 the replacement of thiophene with selenophene results in a reduction of the optical bandgap due to the increase of quinoid character in the polymer backbone.148-150 In a closer look of the film absorptions, it is also found that the full width at half-maximum (FWHM) of PCDSeBT (155 nm) is wider than that of PDCTBT (140 nm), as a matter of a characteristic of strong intermolecular Se···Se interactions, which can potentially further increase JSC value. The electrochemical properties of PCDSeBT were investigated by cyclic voltammetry (CV). As shown in Figure 2.3.1b, PCDSeBT exhibits clear reversible n-doping/dedoping processes in the negative potential range, whereas quasi-reversible p-doping/dedoping behaviors in the positive potential range are observed. The HOMO and LUMO energy levels are estimated to be −5.40 eV and −3.70 eV, respectively, using the ferrocene-ferrocenium (Fc/Fc+) redox couple (4.8 eV below the vacuum level). Both PCDTBT and PCDSeBT have nearly identical HOMO energy levels, but PCDSeBT exhibits 0.10 eV lower-lying LUMO level relative to PCDTBT (LUMO = −3.60 eV), verifying our presumption about the effect of selenium on the selective fine-tuning of LUMO level. The material-design rules described by Scharber et al.151 Suggested that the PCEs of a BHJ solar cell should be much more sensitive to changes of the donor LUMO level compared to variations of the donor bandgap. On the basis of the rules, the estimated PCE from the Eg opt and the LUMO value of PCDSeBT is 7.8%. This theoretical value is much higher than that of PCDTBT (6.5%), indicating that a highly promising material for PSCs considering the frontier orbital energies. Upon utilizing a model dimeric system containing methyl groups, the optimized molecular geometry of PCDSeBT and its frontier molecular orbitals of the calculated HOMO and LUMO iso-surfaces were computed by density functional theory (DFT, B3LYP/6-31G) (Figure 2.3.1d). The HOMO of PCDSeBT is well-distributed along the conjugated chains; its LUMO is mainly centralized on BT accepting core as shaped by orbital lobes, being predicted a p-type organic semiconductor. In order to corroborate the effect of the heteroatom substitution on charge transporting properties of the polymers, top-contact organic field- effect transistors (OFETs) were fabricated using solution processed PCDTBT and PCDSeBT, respectively, as the semiconducting layer on the octadecyltrichlorosilane (OTS) self-assembled monolayer (SAM)-modified Si/SiO2 substrates (see the detailed devices fabrication in the Experimental Section). The OFET mobilities are calculated in the saturation regime using the following equation: Ids
= (W/2L) × μ × Ci (Vgs − Vth)2, where W and L are the channel width and length, respectively, Ci is the capacitance per unit area of the insulation layer. Linear plot of Ids 1/2 vs Vgs deduced from the Ids vs Vgs measurement. These devices show characteristics of a typical p-channel transistor with good drain- current Modulation, well-defined linear, and saturation regions (Figure 2.3.2). The summary of the performances is provided in Table 2.3.1. The OFET device using as-cast PCDTBT films without
thermal annealing exhibits a hole mobility of 2.2 × 10−4 cm2/V·s with an on/off current ratio (Ion/Ioff) of 4.44 × 103. For PCDTBT thin films after annealing at evaluated temperatures the mobilities are not markedly improved, implying that the PCDTBT thin films remain nearly amorphous for both as-cast and annealing at high temperature.
Figure 2. 3. 2. Transfer characteristics of (a) PCDTBT- and (b) PCDSeBT-based OFET devices at different annealing temperatures.
On the other hand, it is found that the unannealed thin films of PCDSeBT exhibit a slightly higher mobility of μh = 5.1 × 10−4 cm2 /V·s, compared with that of pristine PCDTBT. Interestingly, in contrast, as the PCDSeBT thin films are annealed at a temperature of 120 and 150 °C, the mobilities are systematically improved up to 1.0 × 10−3 cm2 /V·s (Figure 2.3.2b), which is about 1 order of magnitude higher than that of PCDTBT, possibly due to increased interpolymer chain contact induced by Se···Se interactions with the thermal annealing process.
Table 2. 3. 1. OFET performance of PCDTBT and PCDSeBT polymer thin films at different annealing temperatures
(μh)(cm2/V.s) Ion/Ioff Vth[V]
As-cast 2.2 Ⅹ 10-4 4.4 Ⅹ 103 -21
120℃ 4.9 Ⅹ 10-4 7.9 Ⅹ 103 -22
150℃ 3.5 Ⅹ 10-4 7.9 Ⅹ 103 -34
As-cast 5.1 Ⅹ 10-4 4.1 Ⅹ 104 -19
120℃ 7.8 Ⅹ 10-4 3.4 Ⅹ 104 -9
150℃ 1.0 Ⅹ 10-3 4.0 Ⅹ 104 -13
Figure 2. 3. 3. X-ray diffraction patterns of PCDTBT(a) and PCDSeBT(b) thin films before (i) and after annealed at 150 °C (ii).
To gain a better understanding of the influence of the thermal annealing, the crystallinity and molecular organization of PCDTBT and PCDSeBT thin films were investigated by X-ray diffraction (XRD), both before and after annealing at 150 °C. Both the as-cast and annealed PCDTBT thin films fail to reveal any defined scattering patterns (Figure 2.3.3a), indicating the macroscopically disordered, amorphous structure. In the case of PCDSeBT, the as-cast thin films show very weak diffractions
(Figure 2.3.3b). Upon thermal annealing, the primary peak at 4.42°, corresponding to a d-spacing of 19.99 Å, progressively intensifies and the secondary broad peak at ∼21.1° (d = 4.21 Å) that is probably related to π−π stacking becomes visible (Figure 2.3.3b). On the basis of these XRD results, we can conclude that the oriented microstructure of the as-cast PCDSeBT thin films is kinetically limited but the polymer chains reorganize to ordered lamellar packing structures upon annealing. This observation is a plausible explanation for the sudden rise in mobility of PCDSeBT as a function of the thermal annealing.
Photovoltaic effects of PCDSeBT were investigated in BHJ PSCs with the device structures of the standard configuration glass/ITO/PEDOT:PSS/PCDSeBT:PC71BM/Al. The PCDSeBT:PC71BM weight ratio was optimized from 1:1, 1:2, 1:3, to 1:4. The current-density−voltage (J−V) characteristics of the devices under the illumination of simulated AM 1.5G conditions (100 mW/cm2) are shown in Figure 2.3.4a and the parameters are summarized in Table 2.3.2. Without extensive optimization, the initial device fabricated from the blend solutions with a PCDSeBT:PC71BM weight ratio of 1:1 shows a PCE of 0.73% with a JSC of 2.98 mA/cm2 , a VOC of 0.71 V, a fill factor (FF) of 35%. As increasing the weight fraction of PC71BM, the PCEs are gradually increased. The device containing the 1:4 w/w blend as the photoactive layer after thermal annealing at 150 °C delivers at superior performance with the JSC of 11.7 mA/cm2 , VOC of 0.79 V, and FF of 45%, improving the PCE to 4.12%, an approximately 37% enhancement in PCE, when compared to the reference cell based on PCDTBT:PC71BM for the sake of comparison (see Figure 2.3.4c).
Table 2. 3. 2. Photovoltaic properties of PSCs based in PCDSeBT.
1:1 2.98 0.71 0.35 0.73
1:2 4.66 0.76 0.42 1.50
1:3 9.97 0.79 0.46 3.64
1:4 11.7 0.79 0.45 4.12
(before thermal annealing) 10.3 0.64 0.42 2.76
Figure 2. 3. 4. J–V characteristics of PSCs based on PCDSeBT:PC71BM under illumination of AM 1.5 G, 100 mW/cm2 (a). Incident photon-to-current efficiency (IPCE) spectrum of PCDSeBT:PC71BM (1:4 w/w)-based device (b). Reference device with PCDTBT:PC71BM (c).
It is worth noting that the JSC, to the best of our knowledge, is among the highest JSCs reported to date for PCSs based on PCDTBT analogues,152 in a good agreement with the extended absorption of sunlight through the low bandgap and broaden absorption band of PCDSeBT. In order to ensure the accuracy of the measurements, we investigated the incident photon-to-current efficiency (IPCE) spectrum of the optimized device (1:4 w/w), exhibiting over 65% at the energetically lower peak, i.e. at the λ max of PCDSeBT (Figure 2.3.4b).
Figure 2. 3. 5. AFM images (6 μm × 6 μm) of PCDSeBT:PC71BM (1:4 w/w) cells before (a) and after (b) thermal annealing at 150 °C, respectively.
The JSC value calculated by integrating the IPCE data with an AM 1.5G reference spectrum is rather consistent with that obtained from J−V plots within 10% error. Atomic force microscopy (AFM) was performed to gain insight into the surface morphology of the optimized 1:4 w/w blend films (Figure 2.3.5). The films before and after thermal annealing have smooth surface topographies and very similar features, where the formation of voids, typically attributed to incompatibility between donor and acceptor components, is not observed. However, the rms roughness is somewhat reduced to from 0.47 to 0.43 nm with thermal treatment, being favorable for charge separation and transport. This can reasonably explain the enhanced efficiency via the post-annealing effect. Note that, in stark contrast to PCDTBT:PC71BM system in which thermal annealing reduced the photovoltaic parameters (FF, JSC, and VOC),153 the performance of all PCDSeBT-based devices for this study is considerably improved as a result of thermal treatment. We can conclude that the formation of crystalline nanoscale domains would be slightly induced in PCDSeBT:PC71BM with a thermal treatment in consequence of the ordered crystalline nature of the PCDSeBT on annealing as supported by the XRD results above as well as the large quinoidal character in the polymer backbone as the inclusion of selenophene.154 The AFM of the annealed film gives an evidence for slightly nanofibril-like organization (see Figure 2.3.5b).
Figure 2. 3. 6. Measured J–V characteristics by the space charge limited current (SCLC) method with PCDSeBT:PC71BM (1:4 w/w) films under dark conditions before and after thermal annealing for hole-only device (a) and electron-only device (b).
The hole and electron mobilities of PCDSeBT:PC71BM (1:4 w/w) blends were measured using the space-charge-limited current (SCLC) method and the J−V characteristics were plotted in Figure 2.3.6.
The hole mobility (μ hole = 4.68 × 10−5 cm2 /V·s) obtained with the thermally annealed film is one order higher than that without post annealing (μ hole = 4.02 × 10−6 cm2 /V·s), whereas in the both cases, the electron mobilities (μ electron) are similar (1.24 × 10−3 and 5.58 × 10−3 cm2 /V·s) for as- cast and annealed films, respectively, yielding a smaller difference between the mobility ratio for the annealed film. The higher mobilities and more balanced charge transport should definitely favor the charge transportation in the blend film and lead to high solar cell performance, supporting the beneficial effect of the thermal annealing on PCDSeBT:PC71BM cells.